Electrodeless Measurement Technique of Complex Dielectric
Permittivity of High-K Dielectric Films in the Millimeter
Igor Kotelnikov1, *, Andrey Altynnikov1, 2, Anatoly Mikhaylov1, Valentina Medvedeva1, and Andrey Kozyrev1, 2
Abstract—An electrodeless measurement technique of complex dielectric permittivity of high-K dielectric ﬁlms is described. The technique is based on a quasi-optic Fabry-Perot resonator and modiﬁed for investigation of two-layer dielectric structures — substrate/K-ﬁlm. This procedure is destined to be used for providing a simple intermediate control of parameters of high-K ﬁlms before the following technological process. Regimes of measurements providing the most sensitive conditions for deﬁnition of ﬁlm parameters are considered. The proposed method is tested on two-layer structures with well-known parameters and is used for characterization of ferroelectric (Ba,Sr)TiO3 ﬁlms in the millimeter
wavelength range (∼50 GHz).
The characterization of microwave parameters of dielectric ﬁlms with elevated values of the permittivity is required for diﬀerent types of microwave (MW) devices (MOSFET, MEM RF switches, MW-photonic elements-electro-optic modulators etc.). The development of technology required to create new materials and components for MW devices is associated with instruments adapted for fast and accurate MW measurement in order to control the parameters of the developed structures and to correct processing methods for their preparation.
One of the broadly used class of measurement procedures of high-K dielectric ﬁlms is the measurement of metal/dielectric/metal (M/D/M) structures, which may be in the form of electrodynamically lumped (capacitors) or distributed (strip or coplanar lines and resonators) elements [1, 2]. The main disadvantages of this method are the uncertainty in the impact of the technological process of metal deposition on intrinsic (original) properties of dielectric ﬁlm, and the problem of separation of microwave losses in dielectric, M/D interfaces and metal electrodes.
In order to avoid the above drawbacks, it is reasonable to use electrodeless measurements which allow characterization of the ﬁlm itself, before the following technological process of subsequent layers deposition. To provide the electrodeless measurements of the dielectric permittivity (ε) and dielectric loss tangent (tanδ) of materials at microwave frequencies the metal cavity resonators are widely used [1– 4]. However, for the millimeter and especially sub-millimeter wavelengths, the above method is faced with considerable diﬃculties: (i) the microwave surface resistance of cavity metal walls increases at higher frequencies that leads to the decrease of the quality (Q) factor of the resonator, i.e., the accuracy of measurements decreases, (ii) the installation of the tested sample into the cavity usually involves disassembling and reassembling which if done frequently inevitably results in a variation of resonator
Received 5 October 2016, Accepted 24 November 2016, Scheduled 8 December 2016
* Corresponding author: Igor V. Kotelnikov (firstname.lastname@example.org).
1 Saint-Petersburg Electrotechnical University, Saint-Petersburg 197376, Russia. 2 Dagestan University of National Economy,
parameters, that in turn leads to the need for permanent calibration of the resonator, (iii) the frequency density of diﬀerent resonance modes of the cavity is very high and the identiﬁcation of the mode required is rather a complicated problem.
One of the most promising methods without the mentioned drawbacks is the use of the open quasi-optic Fabry-Perot resonator (hereinafter OR). OR are used on MW up to hundreds GHz  for deﬁnition of electrodynamical parameters of solid substances, gases and plasma. In accordance with  the Q-factor for empty OR operating at millimeter wave frequencies is typically in the range (1–2)×105 and can be increased by a factor of ∼ 5 employing so-called Bragg reﬂectors . There are a set of works devoted to measurements of the complex dielectric permittivity on the base of OR. In  the measurements of one-layer materials with low values ofε(quartz and Teﬂon disks) are presented at 20– 40 GHz. The aim of the work is to determine the measurement error as a function of disk diameter. In  the possibility of very precise measurements at Ka band is demonstrated for a set of one layer dielectric materials with ε < 10. Note that many of recent works are devoted to increasing the measurement’s accuracy of electrodynamic parameters of one layer solid materials with low dielectric constant [9–11].
In , the theory of OR for measurements of multilayer dielectric structure is well developed, and its correctness is conﬁrmed by 35 GHz measurements of a two-layer structure (Al2O3
substrate/(Ba,Sr)TiO3ﬁlm) with thickness of (Ba,Sr)TiO3 (BSTO) ﬁlm ∼ 50µm. Our present work
which is based on the practically classical approach of [5, 6, 12, 13] is focused on a more detailed consideration of the most sensitive regimes of measurements corresponding to diﬀerent values of substrate thicknesses and dielectric constant of the high K-ﬁlm.
The proposed method is tested on two-layer structures with known parameters (SiO2, LaAlO3,
Al2O3) and is used for deﬁnition of parameters of ferroelectric BSTO ﬁlms (thickness∼5µm,ε >400)at
frequency∼50 GHz. This procedure is destined to be used for providing a simple intermediate control of parameters of high-K ﬁlms before the following technological processes.
2. THEORETICAL ASPECTS
The schematic of OR with the sample located on the ﬂat mirror is presented in Fig. 1. The sample is a two-layer structure — substrate/high K-ﬁlm. The microwave properties of substrate are known from handbooks or on the base of preliminary measurement of the substrate without ﬁlm in open resonator. Installation of the sample changes the resonance frequency and to restore the mode of measurements the frequency shift is compensated by the movement of the plane mirror at a distancep. Theoretical approach of measurements is based on results of theory developed by  for E- and H-ﬁeld distribution in open resonator with one layer dielectric. Relationship between the resonance frequency
Input and output coupling
(f) and the permittivity of the ﬁlm (εf) on the substrate (εs) can be obtained on the base of boundary condition equations for three areas of material (substrate/ﬁlm/air) between metal mirrors of OR and impedance transformation approach (see for example ). Solution of the system of equations results in a transcendental equation, which provides the relation between resonance frequency and permittivity of the ﬁlm:
εf · 1
εskt+ √1 εf tan
εf − 1
=−tan (kd+ Ψ), (1)
where: t and a — thicknesses of substrate and the ﬁlm respectively, k — the propagation constant in the free space, ψ – the value correcting the phase shift at the plane mirror taking into account the spherical shape of the wave front (see in ), d=D−p−t−ais the distance between mirrors with sample after the resonator adjusting on resonance frequency of empty OR.
The deﬁnition of εf allows to deﬁne the so-called coeﬃcient of the ﬁlm inclusion (electric energy ﬁlling factor) (ξf) in the resonator. The coeﬃcient is deﬁned as the ratio of electric ﬁeld energy stored in the ﬁlm to the total energy of the electric ﬁeld stored in the resonator:
ξf = Wf
whereWf,WsandWa— energies of the electric ﬁeld stored in the ﬁlm, the substrate and the air regions respectively. These values are calculated by the volume integration of the E-ﬁelds strength distribution in OR with sample.
On the base of the simplest equivalent circuit presentation of the resonator, the dielectric losses of the ﬁlm located on the substrate can be deﬁned as:
tanδf = ξ1 f
1 Q0 −
where: Q0 — the unloaded quality factor of the open resonator with substrate/ﬁlm sample, Q00 —
the unloaded Q-factor of the empty resonator without sample,ξs — coeﬃcient of the inclusion for the substrate, which is deﬁned by equation analogical to (2), tanδs — dielectric losses in the substrate.
It is clear from Eq. (3) that the correct deﬁnition of inclusion coeﬃcients (ξs,ξf) plays a dominant role in the procedure of measurements. At ﬁrst glance, it would seem that the increase of the thickness of the substrate without ﬁlm must result in an increase of the inclusion coeﬃcient of substrate. However, experimental and modeling data demonstrate the periodicξs(d) dependence (Fig. 2), which is
t, 0.00 0.25 0.50 0.75 1.00 1.25 1.50 s 0.00 0.05 0.10 λ ξ
explained by the periodically changing of E-ﬁeld coupling between substrate and air arias. Calculation demonstrates that maximums ofξs(d) dependence corresponds to the maximums E-ﬁelds strength at the substrate surface, that is the most sensitive regime for measurements of ﬁlm located on the substrate. This fact is illustrated by ξf(εf) dependences (Figs. 3(a), (b)) for ﬁlms of diﬀerent thicknesses located on the substrate with electrical thicknesses λ/4 and λ/2. The thickness of (2n−1)λ/2 (where n is an integer) provides a minimum of the electric ﬁeld at the substrate-ﬁlm boundary, and accordingly, the lowest value of inclusion coeﬃcient in comparison with (2n−1)λ/4 conditions. One can conclude that to provide the most accurate measurement of ﬁlm parameters (εf, tanδf) after the preliminary substrate measurement without ﬁlm (εs, tanδs), the ﬁnal ﬁlm measurements must be done at frequencies corresponding to (2n−1)λ/4 conditions for the substrates. If the thickness of the substrate does not correspond to the condition of maximum sensitivity of measurements of the ﬁlm, the additional layer of substrate material of required thickness must be located on the metal mirror under the substrate/ﬁlm structure.
200 400 600 800 1000
0.0000 0.0002 0.0004 0.0006 0.0008
200 400 600 800 1000
0.000 0.001 0.002 0.003 0.004 0.005 0.006
0.5μm 2μm 5μm
Figure 3. Inclusion coeﬃcient of the ﬁlm as a function of it’s permittivity at diﬀerent ﬁlm thicknesses. Substrate (ε= 10) with thickness (a) λ/4 and (b) λ/2.
OR used in experiments is characterized by the following parameters: plane mirror diameter 120 mm, diameter aperture of concave mirror 200 mm and its curvature is of 139 mm. OR is destined to be used in the frequency range off = (40÷75) GHz. Unloaded quality factor of the empty OR is ofQ00(60 GHz)
= (5–6)×104. The ﬂat mirror movement is provided by the micrometer scale mechanical screw. Mode TEM00q was used for investigation. The mode identiﬁcation is done by |S21| measurements of OR
at diﬀerent positions of small disturbing absorber ball (∅1.0 mm) above the ﬂat mirror. Correctness of Eqs. (1) and (3) to deﬁne the parameters of the ﬁlm layer on the substrate was conﬁrmed by the measurements of structures consisting of two layers with well-known MW parameters of each layer. For samples containing the diﬀerent combination of layers (SiO2, LaAlO3, Al2O3) with scale of thicknesses
(0.2÷1.5) mm) the simulation of parameters of layer which was considered as an “unknown layer” have been done on the base of our measurements and Eqs. (1), (3) in the frequency range (45÷70) GHz. For these “unknown layers” the errors of ε and tanδ in comparison with handbooks data were not more than 1% and 5% respectively.
Results of the measurements at frequency ∼50 GHz of three types of (Ba0.5Sr0.5)TiO3 ﬁlms with
diﬀerent concentration of Mg2TiO4 dopants  and with thickness of 5µm on MgO substrate (0.5 mm)
Figure 4. Results of electrodeless measurements ((a) εf and (b) tanδf) of three types of (Ba0.5Sr0.5)TiO3 ﬁlms with diﬀerent dopant concentration at frequency ∼ 50 GHz (red icons) and
generalized frequency dependences of dielectric parameters of ﬁlms (violet ﬁlling — guide for eyes).
Theoretical dependences of inclusion coeﬃcients (ξs, ξf) (Figs. 2, 3) were used to provide the most sensitive regimes of measurements. Operation frequency and substrate thickness correspond to conditions close to the ﬁrst maximum of ξs(t) (Fig. 2) that determines the value ofξf = 0.003÷0.005 for 5µm K-ﬁlms withε= (400÷800) (Fig. 3(a)). The unloaded Q factor of OR with diﬀerent samples corresponds toQ0 = 3500–5000. Note that for high-K ﬁlms with signiﬁcantly higher tanδthe use of the
measurement regimes close to maximums of dependencies ξs(t) are problematic due to degradation of OR resonance. In this case for reliable visualization of resonance curve it is necessary to use the regime corresponding to lower values of ξs and ξf, that is the range between maximum and minimum ofξs(t) dependence. Obviously that results in decrease of accuracy of measurements.
ferroelectrics [17, 18]. The results of electrodeless measurements of dielectric losses also correspond to nature of ferroelectrics: the higher dielectric constant — the higher the dielectric losses.
The main source of basic errors is connected with correct deﬁnition of the ﬁlm inclusion coeﬃcient and in accordance with our simulation for the most critical situation corresponding to thin ﬁlm (0.5µm) with low permittivity (εf = 100) the relative errors are not more than Δεf/εf = 5% and Δ tanδf/tanδf = 10%. For thick ﬁlms (≥10µm) with the same permittivity the errors are less than 2% for permittivity and 5% for losses.
The developed technique based on the quasi-optical Fabry-Perot resonator provides the dielectric constant and dielectric loss tangent measurements of high-K ﬁlms deposited on the substrate in the mm-wave frequency range with a rather high accuracy. To provide the most accurate measurement of ﬁlm parameters (εf, tanδf), the measurements must be done at frequencies corresponding to (2n−1)λ/4 conditions for the thickness of substrates. The developed technique can be used for both the laboratory study of high-K ﬁlms and due to its simplicity for fast (express) control measurements in serial production. Results of measurements of BSTO ﬁlm parameters (ε, tanδ) at frequency∼50 GHz can be interesting for designers of ferroelectric MW devices.
This work was supported by the Ministry of Education and Science of the Russian Federation in the framework of “Research and development in priority areas of advancement of the Russian scientiﬁc and technological complex for 2014–2020”, agreement No. 14.608.21.0002 of 27.10.2015 (unique number of agreement RFMEFI60815X0002).
1. Chen, L. F., C. K. Ong, C. P. Neo, V. V. Varadan, and V. K. Varadan, Microwave Electronics. Measurement and Materials Characterization, John Wiley & Sons, Ltd., 2004.
2. Spartak, G., Ferroelectrics in Microwave Devices, Circuits and Systems: Physics, Modeling, Fabrication and Measurements, Springer Science & Business Media, 2009.
3. Jerzy, K., “Frequency domain complex permittivity measurements at microwave frequencies,” Measurement Science and Technolpgy, Institute of Physics, Meas. Sci. Technol., 17, 2006.
4. Lee, C.-S. and C.-L. Yang, “Thickness and permittivity measurement in multi-layered dielectric structures using complementary split-ring resonators,” IEEE Sensors Journal, Vol. 14, No. 3, March 2014.
5. Clarke, R. N. and C. B. Rosenberg, “Fabry-Perot and open resonators at microwave and millimeter wave frequencies, 2–300 GHz,”Journal of Physics E: Scientific Instruments, Vol. 15, 1982.
6. Krupka, J., A. Cwikla, M. Mrozowski, R. N. Clarke, and M. E. Tobar, “High Q-factor microwave Fabry-Perot resonator with distributed Bragg reﬂectors,”IEEE Trans. Ultrason. Ferroelectr. Freq. Control, Vol. 52. 2005.
7. Yao, Y., H. Cui, J. Wang, E. Li, and B. Tao, “Broadband measurement of complex permittivity by an open resonator at 20–40 GHz,”International Conference on IEEE Communication Problem-Solving (ICCP), 2014.
8. Gui, Y. F., W. B. Dou, P. G. Su, and K. Yin, “Improvement of open resonator technique for dielectric measurement at millimeter wavelengths,” IET Microw. Antennas Propag., Vol. 3, No. 7, 2009.
10. Hong, Y.-P., H. Koo, and M. J. Salter, “Measurement of high-permittivity dielectric characteristics at microwave and mm-wave frequencies,” Conference on Precision Electromagnetic Measurements (CPEM 2016), July 2016.
11. Quan, W., D. J. Downing, and M. NurulAfsar, “A signal processing approach for recovery of precision high-Q dielectric resonance proﬁle measurements,” 2016 Conference on Precision Electromagnetic Measurements (CPEM 2016), July 2016.
12. Anatoli, D. and G. Spartak, “Open resonator technique for measuring multilayered dielectric plates,” IEEE Transactions on Microwave Theory and Techniques, Vol. 53, No. 9, 2005.
13. Yu, P. K. and A. L. Cullen, “Measurement of permittivity by means of an open resonator,”Proc. R. Soc. London: Ser. A., Vol. 380, 1982.
14. David, P., Microwave Engineering, 4th Edition, John Wiley & Sons Inc., 2012.
15. Cullen, A. L., “Millimeter-wave open-resonator techniques,”International Journal of Infrared and Millimeter Waves, Vol. 10, Springer, 1983.
16. Andrey, K., K. Alexei, N. Elizaveta, O. Vitaly, and K. Dmitry, “Observation of an anomalous correlation between permittivity and tunability of a doped (Ba,Sr)TiO3 ferroelectric ceramic
developed for microwave applications,”Applied Physics Letters, Vol. 95, 012908, 2009.
17. Vendik, O. G. and S. P. Zubko, “Ferroelectric phase transition and maximum dielectric permittivity of displacement type ferroelectrics (BaxSr1−xTiO3),” Journal of Applied Physics, Vol. 88, 5343,